Optical Properties Of Solids

Author
enareshkumar23 
Category
Documents

view
215 
download
16
Embed Size (px)
description
Transcript of Optical Properties Of Solids
OPTICAL PROPERTIES OF SOLIDS
OPTICAL PROPERTIES
OF SOLIDSFrederick.
Wooten
Department of Applied ScienceUniversity of CaliforniaDavis, California
1972
ACADEMIC PRESS
New York and London
soJjfc
ia
Copyright 1972, by Academic Press, Inc. all rights reserved no part of this book may be reproduced in any form, by photostat, microfilm, retrieval system, or any other means, without written permission from the publishers.
ACADEMIC
Ill Fifth Avenue,
PRESS, INC. New York, New York
10003
ACADEMIC
United Kingdom Edition published by
PRESS, INC.
24/28 Oval Road, London
NW1
(LONDON) LTD.
Library of Congress Catalog Card Number: 72187257
PRINTED IN THE UNITED STATES OF AMERICA
To
My
Father
CONTENTSPreface
A cknowledgments
Chapter
1
Introductionl.i
Band Theory of SolidsOptical Reflectivity
1.2 1.3
PhotoemissionCharacteristic Energy Loss Spectra14
1.4
Chapter 2
Maxwell's Equations and the Dielectric Function2.1
Maxwell's Microscopic Equations Maxwell's Macroscopic Equations
16 16
2.2 2.3
Formal Solutions of Maxwell's EquationsAnalysis of Charge and Current DensitiesProperties of the
18
2.42.5
2225
Medium
2.62.7 2.8
Interaction of Light with the
Medium
26
External Sources and Induced Responses
2931
Fourier Analysis of Maxwell's Equations
2.9
The
Dielectric Tensor Problems Further Reading
3439
4
Chapter
3
Absorption and Dispersion3.1
The Lorentz
Oscillatorfor Metals
425255
3.23.3
The Drude Model
A Qualitative Look atQuantum Theory
Real Metals
3.43.5
Photoemission from Copperof Absorption and Dispersion
6667
vii
1
Vlll
Contents
3.6 3.7 3.8
Oscillator Strengths
and
Sum
Rules
7275
Applications of
Sum
Rules
The Absorption
Coefficient, Optical Conductivity,
and80g2
Dielectric Function Problems Further Reading
84
Chapter 4
FreeElectron Metals4.1
Classical
Theory of FreeElectron Metals
86
4.2 4.3
The
Classical Skin EffectEffect
90
The Anomalous SkinProblems
9499j
4.4
Optical Properties and the Fermi Surface
Qg
References and Further Reading
107
Chapter 5
Interband Transitions5.1
Periodic PerturbationDirect Interband TransitionsJoint Density of States and Critical Points
108
5.25.3
110116122
5.45.5
Direct Transitions in
Germanium
Direct Transitions in Silver: Effects of Temperature and
Alloying5.6 5.75.8
Indirect Transitions
j
34
The Absorption EdgeExcitons
in
Ge, AgBr, and AgBr(Cl)
144149153
5.9
Direct and Indirect Transitions in Photoemission
5.105.1
Nondirect Transitions: Photoemission from Cs 3 BiTransport and Escape Cone Effects on Photoemission
1561
59
5.12
Photoemission and Electron Transport Problems Further ReadingReferences
in
Al and
GaAs
1641
(39
1
70
171
Chapter 6
Dispersion Relations and6.1
Sum
Rules
Linear Response Functions and KramersKronig RelationsReflectivity
173181
6.2 6.3
and Phase
Shift Dispersion Relations
Sum
Rules
182
Problems Further Reading
1841
85
Contents
IX
Chapter 7
SelfConsistent Field Approximation7.1
SelfConsistent Field ApproximationSpecial Cases
186
7.2
and Applications
194201
ProblemsReferences and Further Reading
202
Chapter 8
CurrentCurrent Correlations and the FluctuationDissipation8.1
Theorem204206 207 209 209
Transition Rate and CurrentCurrent Correlations
8.28.3
Current Fluctuations
The FluctuationDissipation Theorem and theConductivity
ProblemReferences and Further Reading
Chapter 9
Plasmons and Characteristic Energy Losses9.1
SingleElectron Excitations in Metals
211
9.29.3
Plasmons
in
Simple Metals
214215
The Plasmon Cutoff Wave VectorCharacteristic Energy Loss Spectra
9.49.5
218
Surface Plasmons
ProblemsReferences and Further Reading
220 223
224
Appendix
A
Decomposition of a Vector Field into Longitudinal and Transverse Parts
225
Appendix BB.l
The Local
Field227
Insulators
B.2
Nonlocalized ElectronsFurther Reading
230231
Appendix
C
Reflection at
Normal Incidencefor a Crystal
232
Appendix
D
The /Sum Rule
234
Appendix E
Interaction of Radiation with Matter
236
Contents
Appendix F
M
t
Critical Points
240
Appendix
G
Reflectance and PhaseShift Dispersion RelationsG. 1
The PhaseShift Dispersion RelationNumerical Integration of the PhaseShift Equation Further Reading
244248
G.2
250
Appendix
H
k p Perturbation Theory
251
Index
255
PREFACEThe present book attempts to fill a need for a fundamental textbook which explains the optical properties of solids. It is based on two short courses I gave in the Department of Applied Science and a series of fifteen lectures at Chalmers Tekniska Hogskola, Goteborg, Sweden presented at the invitation of Professors Stig Hagstrom, Gosta Brogren, and H. P. Myers. This book is meant to explain a number of important concepts rather than present a complete survey of experimental data. Its emphasis is almost entirely on intrinsic optical properties and photoelectric emission. Little is said concerning imperfections, color centers, etc. However, the principles are general, so the book serves as a stepping stone to the more advanced review articles and papers on a wide variety of topics. The book assumes a background in quantum mechanics, solid state physics, and electromagnetic theory at about the level of a senioryear undergraduate or firstyear graduate student in physics. Problems and exercises have been included to elaborate more fully on some aspectsof the physics, to gain familiarity with typical characteristics of optical properties, and to develop some skills in mathematical techniques. The central theme of the book is the dielectric function (a macroscopicquantity)
and
its
properties of solids.
relationship to the fundamental microscopic electronic The emphasis is on basic principles, often illustrated
by simple models. The necessary mathematics needed to understand the models is generally carried through to completion, with no steps missing, and no "it can be shown" statements. Thus, the text is intended to be suitablefor selfstudy, as well as for use in a onesemester firstyear graduate course.
XI
ACKNOWLEDGMENTSThere are many people who have contributed in some way to the making I thank especially those who have permitted the use of their figures from published work. In a more direct personal way, Dr. Louis F. Wouters first aroused in me a latent interest in light and the photoelectric effect and provided the opportunity for my initial research on photoelectric emission. I am grateful to Dr. James E. Carothers and Dr. Jack N. Shearer for their encouragement and support over the years. Dr. Tony Huen, my friend and colleague, aided substantially with many helpful discussions in our daytoday collaboration. Others whom I thank for helpful discusof this book.sions are Professor William E. Spicer, Dr. Erkki Pajanne, Dr. Birger Bergersen, Professor Lars Hedin, Professor Stig Lundquist, Dr. PerOlov Nilsson, Major L. P. Mosteller, Dr. Geoffrey B. Irani, Captain Harry V.
Winsor,Brust.
Lt. George Fuller, Professor ChingYao Fong, and Dr. David Thanks also to Mrs. Peggy Riley, Mrs. Kathryn Smith, and Mrs.
Donna Marshall who
typed parts of the manuscript.
xu
Chapter 1
INTRODUCTION
of solids.
This book presents an introduction to the fundamental optical spectra The aim is to develop an understanding of the relationship of measurable optical properties to the dielectric function and the microscopic
electronic structure of solids.
The usual way to determine the optical properties of a solid is to shine monochromatic light onto an appropriate sample and then to measurethe reflectance or transmittance of the sample as a function of photon energy. Other methods, such as ellipsometry, are sometimes used. However, these methods are of no concern here. The choice of experimental technique information obtained. is largely one of convenience, not of the basicshall concentrate
We
on
reflectivity.
methods of data analysis are left which are included in the references throughout the book. One exception incidence reflectance is the inclusion of a discussion of the analysis of normal the KramersKronig equations; but, the importance data with the use ofhere
Details of experimental technique and to other monographs and papers, some of
Kramerslies in the physics and great generality contained in the Kronig equations, not in the experimental techniques for measuring the reflectance at normal incidence. In recent years, photoelectric emission and characteristic energy loss experiments have proven useful as methods of studying electronic band in structure. These experiments are closely related to optical experiments information they provide. They are discussed at various terms of the kind ofpoints throughout the book. There are experimental techniques other than the optical types which
*
Chapter
1
Introduction
provide information on band structure. These include cyclotron resonance, de Haasvan Alphen effect, galvanomagnetic effects, and magnetoacoustic resonance. However, even though often of high accuracy, these experiments yield information pertaining to energy levels only within a few kT of the Fermi surface. Ion neutralization spectroscopy and soft xray emission provide information over a wide energy range, but they have not provenas useful as optical methods.typical
This chapter discusses briefly the kinds of experiments that are most and indicates the kind of information that can be obtained. To provide a framework for discussions of optical measurements, photo1.1
and characteristic energy loss spectra, we begin in Section with a reminder of some of the ideas of band theory, but no more than that. The reader is assumed to have an adequate understanding of the basicelectric emission,
band theory. Next is a brief introduction to optical reflectivity. followed by a discussion of photoelectric emission. Since even an elementary discussion of the physics of photoelectric emission is notideas of
This
is
included in most textbooks on solidstate physics, it is included here. The final section consists of a brief introduction to characteristic energyloss spectra.
For those unfamiliar with the optical spectrum, it is suggested that Table be memorized. Optical data are often presented in terms of frequency or wavelength, but band structure is discussed in terms of energy (eV).1.1Itis
useful to
know how1.1
to convert units easily.
TABLE
Relationship of Wavelength to Energy, Frequency,
and Color
12,400 A >(.fi(0, co)
(2.141,
The point
is
that, to
compare longitudinal and transverseit
dielectric func
necessary that the polarization of the medium be in the same direction, or an equivalent one, for both modes of excitation. This condition is always satisfied in cubic materials;isit
tions in the longwavelength limit,
can sometimes be
satisfied in other materials.
Problems
39
PROBLEMS2.1
Estimate the
maximum
velocity of electrons in a freeelectron metal
having a density typical of real metals. What is a typical maximum velocity for an excited electron when light of wavelength 600 A is used in optical experiments? How important are relativistic corrections to Maxwell'sequations?2.2
Show
that the polarization current does not lead to energy absorption.
2.3
Derive a wave equation for the vector potential
A
in terms of the
properties of the complex dielectric function.2.4 2.5
Derive expressions for n and k as functions of,
e1
and
e2
.
Define a complex conductivity a = a x + ia 2 where a x is the usual real conductivity a that appears in Maxwell's equations. Maxwell's equations, including the properties of the medium, can now be written in termsof a complex conductivity rather than a complex dielectric function. What ,nd is the relationship of a to ? What is the relationship of J (q, co) to E(q, co)in
terms of as corresponding approximately to the band gap, we identify
That the Lorentz model
is
case. The should decrease with increasing band gap. That indeed is the eV, whereas band gaps of Ge, Si and KC1 are, respectively, 0.8, 1.1, and 7.5 and 1.5. the lowfrequency optical dielectric constants are, respectively, 4, 3.5, strong absorption. There may Region II of Figs. 3.33.5 is characterized by
means that also be appreciable reflectivity in this region. That simply k may be high, leading to appreciable reflecalthough the values of n and absorbed in the material. tivity, the light that is not reflected is strongly and the electrons of the insulator respond as if III, co > coIn region greater they were free electrons. This is because the photon energy is much thus has a metallic than the binding energy of the electron. The insulator well into the reflectance. Of course, for good insulators, this region lies observed visually. However, for semivacuumultraviolet and cannot be,
52
Chapter 3
Absorption and Dispersion
E(eV)Fig. 3.7I,
The
spectral
dependence of the reflectance and
dielectric functions of Si.
Regions
II, III,
and
3.4.
and IV correspond to the regions with the same designation shown [H. R. Philipp and H. Ehrenreich, Phys. Rev. 129. 1550 (1963).]like
in Figs. 3.1, 3.3,
conductorsbut
Ge andis
Si,
the
band gap
lies in
the infraredis
and the region
of metallic reflectance
Ge
Thus, and Si have a metallic appearance.in the visible.
KC10.
transparent to the eye,
The onset
of region
called the (o p we find
IV is defined by e t = plasma frequency. From Eq.(o2
This happens at a frequency
(3.14),
assuming
w
f>
w >
T,
= 4nNe 2 /m
(3.27)
3.2
The Drude Model
for
Metalsis
The Drude modelfor insulators simply
for metals
by equating the restoring force
obtained directly from the Lorentz model to zero. The conduction
3.2
The Drude Model
for Metals
53
electrons of a metal are not bound. Furthermore, because thefor a free electronfield actingis
wave functionis
distributed fairly uniformly throughout the metal, theis
on the electron
just the average field. Thus, there
no need
to
make
corrections for the local field.Eqs. (3.14) and (3.15), takingco
From
=
0,
we have1
fi
i
=
!
"
4nNe 2
m
2 7TTF^ + T2 (co)

_ 2_Theorigin of the viscous
^Ne 2mco(co2
T + r2
(
]
)
for a freeelectron metal is the associated with electrical resistivity. In the ordinary scattering of electrons next chapter, when we derive the properties of a freeelectron metal in terms
damping term
of a complex conductivity rather than a complex dielectric function, we shall see that T = t~\ where t is the mean free time between collisions. If we now make the substitution T = t" 1 and use Eq. (3.27), we get from Eqs.,
(3.28)
and
(3.29)
(1
+2
C0 T
2
2)
(3.31)co(\
+ a>V)
Since the
Drude model
is
obtained directly from the Lorentz model
simply by setting co metal should resemble those for an insulator at frequencies greater than As we saw in the preceding section, the frequency range co > co in an co.
equal to zero, the optical properties of a freeelectron
insulator corresponds to the region in which the electrons are effectively free, so that it might be more accurate to say that an insulator respondslike a
metal to photons of energy hco
>
hco
.
and the optical constants for a Drude metal is shown in Figs. 3.83.10. The corresponding reflectivity is shown in Fig. 3.11. It is clear from Fig. 3.11 that for an ideal freeelectron metal, the reflectivity approaches unity below the plasma frequency. Above the plasma frequency, the metal is transparent and the reflectivity decreases rapidly with increasing frequency. That this describes the behavior of real freeelectron metals is shown in Figs. 3.12 and 3.13.
A
plot of the dielectric functions
The plasma frequencyregion.for electrons in metalsis
typically lies in the visible or ultraviolet spectralco
That corresponds to
>
10
15
sec
1.
The meansec.
free collision
time
typically t
%
10"
14
Thus, in the region of the
54
Chapter 3
Absorption and Dispersion
Fig. 3.8
Spectral dependence of e t
and30
e 2 for
a freeelectron metal.
The
calculations are for
the case in which
4nNe 2 /m =
co
2 p
of the ordinate along the positivethat of 2 for the frequency range
eV 2 and hT = 0.02 eV. Note the difference in scale and negative axes. The magnitude of e t is much greater than
=
shown. For hoi
1,
and from Eq.n2
(3.30),
we2)
get(3.32)
=FromFig. 3.9,it is
>
k
:
1

K>2)
clear that n
k just above the plasma frequency and so
Eq. (3.32) simplifies tonfor h(o2
*
1

(co
2
p
/co
(3.33)
plasma frequency, n 0. But what does it mean p that the refractive index is zero? The index of refraction is defined in terms of the phase velocity as v p = c/n. Thus, a zero value for n means an infinite
>
hco
.
Just at the
3.3
A
Qualitative
Look
at Real
Metals
55
j
Fig. 3.9
Spectral dependence of net
from the values ofas
shown
in Fig. 3.4.is,
and k for a freeelectron metal. The curves are calculated given in Fig. 3.8. Regions III and IV correspond to the same regions Region II, the region of strong absorption, is the range ^ tico j 0.02 eVrange
in this case. It
in general, the
^
hco
^
hT. Region
I
does not
exist for metals.
phase velocity and aninfinite
infinite
meansis
the electrons are
wavelength. That the wavelength becomes all oscillating in phase; however, there isas with a true
no polarization charge densitytinction
plasma
oscillation.
The
dis
made
clear in the next section as well as in
Chapter
9.
3.3
A Qualitative Look at Real Metalswill
in a discussion of the Real metals exhibit aspects of both models. To see the role of both models in describing real metals, consider the schematic band diagram for a metal as shown in Fig. 3.14. Two typical transitions are illustrated in Fig. 3.14. The first of these, called an intraband transition, corresponds to the optical excitation of an
We
now
use the Lorentz and
Drude models
optical behavior of
some
real metals.
electron from below the Fermi energy to another state above the Fermi energy but within the same band. These transitions are described by the
56
Chapter 3
Absorption and Dispersion
Drude model. There is no threshold energy for such transitions; however, they can occur only in metals. Insulators do not have partially filled bands that would allow excitation of an electron from a filled state below theFermi energy to an empty state within the same band. That what makes an insulator nonconducting.is,
of course,
The second
transition illustrated in Fig. 3.14
is
a direct interband transi
an electron to another band. It is called a direct or vertical transition because it involves only the excitation of an electron by a photon. Since the momentum of a photon is very small compared with the range of values of crystal momentum in the Brillouin zone,tion. It is the optical excitation of
conservation of total crystal momentum of the electron plus photon means that the value of wave vector k for the electron is essentially unchanged inthe reduced zone scheme. There are nonvertical or indirect transitions between bands, and we shall consider them later; but for present purposes,
a discussion of direct transitionsoptical properties of real metals.
is
sufficient to illustrate the characteristic
Direct interband transitions have a threshold energy. For the
band
1
1
\\
\k\i
n

\
10"
^\n
io

^\kflOJp1 1
10
i
i
i
i
i
i
i
I
i
i
i
ii810II
I
7ficu(eV)
Fig. 3.10
A
semilogarithmic plot of the n and k values for a freeelectron metal as taken
from
Fig. 3.9.
1
3.3
A
Qualitative
Look
at Real
Metals
57
90
^
8070
60 50


4030

1
20
\flGUp
10N.
i
i
i
i
i
i
I
I
1
I
T
I
i
i
l~7
2
3
4
5fico(eV)
6
7
8! F
h
I
1
10
Fig. 3.1
1
Spectral dependence of reflectivity for a freeelectron metal.in Fig. 3.9.
The curve
is
calculated
from the n and k values given
transition
diagram shown in Fig. 3.14, the threshold energy is the energy hco for the from the Fermi energy at k to the same state k in the next higher band. This threshold energy is analogous to that for the excitation of an electron across the band gap in an insulator. Now, how do we use these models to understand real metals, and where do we begin? The beginning is an experimental determination of the reflectance over a wide frequency range. From the reflectance, the dielectricfunction can be obtained using,ine.g.,
a
KramersKronig analysis as discussed
Chapter 6. The dielectric function can then sometimes be split into bound (Lorentz) and free (Drude) contributions and interpreted in terms of the fundamental electronic band structure of the solid. We shall see how this can be done in some cases by following through the steps used by Ehrenreich and Philipp in their classic paper on the optical properties of silver andcopper.
Thevolts
reflectance of silveris
noble metals
is shown in Fig. 3.15. A band diagram shown schematically in Fig. 3.16. The d bands lie
for the
several
below the Fermi energy. Thus, only interband transitions of conduction electrons are possible at low energies, and an onset of interband
~
58
Chapter 3
Absorption and Dispersion
transitions
from the d bands to higherlying conduction band
states takes feasible to
place in the visible or ultraviolet.
separate the dielectric
Under these conditions, function into free and bound parts,sl
it is
= s/ + &2~\~
e1
b
(3.34)
*>2
&2
(3.35)
where e/ and e 2 are described by Eqs. (3.30) and (3.31) and e^ and e 2 b are described by Eqs. (3.14) and (3.15). Band structure effects are included by using an effective mass in these equations rather than using the freeelectron mass. The separation depends upon the fact that s 2 and s 2 b lie in separate spectral regions. Thus, & 2 can be determined by fitting the data at low frequencies to the Drude model using the relaxation time and effective mass as adjustable parameters. Having determined s 2 f (co) in this manner, h s 2 (co) is found by subtracting e 2 (co) from the experimentally determined s 2 (co). Then, as shown in Chapter 6, s^ico) and s^ico) can be determined
1.0
59.4(Exposed to air)
1100
1500Wavelength (A)
1900
Fig. 3.12
Basal plane reflectance of zinc for nonpolarized
light.
The
angles of incidence are
measured with respect to the surface normal. The sample was a single crystal of highpurity zinc cleaved and maintained in a vacuum chamber at pressure less than 10 9 Torr. Note the drastic change in reflectance after exposure to air. This illustrates the importance of careful sample preparation if the measurements are to be useful. A comparison with the best earlier work on reflectance from evaporated thin films [T. M. Jelinek, R. N. Hamm, and E. T. Arakawa, ORNL TM1164 (1965).] is also shown. [From L. P. Mosteller, Jr. and F. Wooten, Phys. Rev. 171,743 (1968).]
3.3
A
Qualitative
Look
at Real
Metals
59
100
9080
^V

i
i
i
^N.R.P.3
I
1
i
i
H.E.Bennett
Madden
70 M.SilverE.J.Ashley
!
L.R.Canfield
i
G.Hass
i
6050
i
i
i 1
i I
4030 2010
iG.Hass J.EjWaylonis1
1
i
8
10
12
14
16
18
20
22
E(eV)
100
~Data of H. E.Ber nett, M.S Iver.a ndE.J .Ashle y
90
850.2
0.4
0.6
0.6
.0
1.2
1.6
1.8
2.0
2.2
E(eV)Fig. 3.13
Reflectance of aluminum.transition.
The decrease
in reflectance at ha>
=
1.4
a
weak interband
The
large decrease in reflectance atR. Philipp,
ha =
14.7
eV arises from eV identifies the
plasma resonance. [From H. Ehrenreich, H.(1963).]
and
B. Segall, Phys. Rev. 132, 1918
b f from a KramersKronig analysis of e 2 ( w ) an d e 2 (co), respectively. The results of such an analysis for silver are shown in Figs. 3.17 and 3.18. The reflectance of silver is high at photon energies below 3.9 eV. At
3.9 eV, the reflectance
drops sharply, then
rises
almost immediately. Theis
reflectance well into the vacuumultraviolet region
characteristic of
interband transitions spread over a wide spectral region. The reflectance of silver near 3.9 eV is striking, but we can interpret this behavior quite simply. The sharp decrease in reflectance at 3.9 eV identifies the plasma frequency. We previously discussed such behavior for
60
Chapter 3
Absorption and Dispersion
*~kFig. 3.14
A
schematic band diagram for a metal. The threshold for direct transitionsat
is
from the Fermi energy
k to the same
state
k
in the next higher
band.
Fig. 3.15Irani, T.
Reflectance of Ag. [From G. B. Huen, and F. Wooten, Phys. Rev.
3B, 2385 (1971).]
4
6
Photon energy (eV)
and we have seen such characteristic behavior aluminum and zinc. In all these cases, the reflectance remained high at photon energies up to the plasma frequency. Then, it dropped sharply where e^ca) passed through zero. The new feature seenanideal freeelectron metalfor the real metals
3.3
A
Qualitative
Look
at Real
Metals
61
Fig. 3.16
Schematic band diagram for the
noble metals.
2
"*
21
Fig. 3.17real
Spectral
dependence
of
the
and imaginaryPhys.
dielectric functions
for Ag.
[From H. Ehrenreich and H.Rev. 128, 1622
R.
Philipp,
(1962).]
2,'
41015
20
25
ficu(eV)
for silver
is
a rapidthat,
rise in reflectance just
To understand
we mustplasmathat a
briefly reconsider
Weit
shall consider
oscillations in
above the plasma frequency. plasma oscillations. detail in Chapter 9. For now,is
is
sufficient to
knowif
plasma
oscillation
a collective oscillation
of the electrons. (See Fig. 3.19.) These oscillations are approximately normal
modes
of the system
they are only weakly damped.itself in
Now, an
oscillation
is
a normal mode if it Thus, we must have
can maintain
the absence of an external
field.
E ext = D  eE =The
(3.36)
acts as a restoring force for the oscillations. Since
net charge separation in the electron gas produces the field E which E j= 0, the condition foroscillationsis
plasma
2
=
,
+
ie,
=
(3.37)
with e 2 go. However, it is a forced oscillation of the system. It exists only in the presence of an external electromagnetic driving force. Thusthe
when one speaksit
of the plasma resonance in the context of optical studies,
refers to this externally forced collective oscillation,
but
it is
not a true
plasma
oscillation.
The
true
plasma
oscillation
is
a cooperative collective
oscillation that persists even after the external field
because, as illustrated in Fig. 3.19, thereoscillation.
is
is removed. This is a mechanism for sustaining the
Now the unusual behavior of Ag is understandable. The sharp decrease ineV is indeed the characteristic decrease at the plasma frequency. However, the reason s^co) passes through zero at hco = 3.9 eV, and not at hco = 9.2 eV as calculated for silver using a freeelectron model,reflectance at 3.9
because of the influence of the d states which lie 4 eV below the Fermi energy in silver. As shown in Fig. 3.18, the effect of the d states is to make a positive contribution to e^co) and so shift to lower energies the point at which e^co) passes through zero. Almost immediately, though, there is ais
3.3
A
Qualitative
Look
at Real
Metals
63
+Ne
Ne
HSx
H8*
equilibrium concentration of electrons
Schematic diagram of the origin of plasma oscillations in one dimension. The is N. The net charge is zero because of a uniform background density of positive ions. Now, imagine that a region of electron charge has been uniformly translated a distance 8x without disturbing the rest of the system. This leaves a region ofFig. 3.19
thickness 8x having a net positive charge density and creates another region of net negative charge density as illustrated in the figure. Because of the force between the two regions of unbalanced charge, they will be attracted toward each other. In the absence of a damping mechanism, there will be an overshoot, leading to the situation depicted in the figure, but with the charges reversed. The system will continue to oscillate in this manner at a characteristic
frequency
known
as the
plasma frequency. Theper unit volume,
oscillations are called
plasma
oscilla
tions.
The plasma frequency can beis
easily derived for this simple case.
Recognizing that the
polarization
the dipole
moment
we have
P =  (NeA 5x)L/AL =  NeSxIn the absence of an external field, this gives rise to the total electric field
E = Theforce
4tiP
= 4nNe 8xis
on an electron
in the
polarized region
thus
mx = eE = AnNe 2 SxThisis
just the equation for a simple
harmonicoi2
oscillator with characteristic frequency
= 4nNe 2 /m
Fig. 3.20
Screening of plasma oscillations by polarization of localized electrons.
Compare
with Fig. 3.19. The d electrons are highly localized on atomic sites. However, their polarizability may be high enough to cause appreciable screening of the forces between fluctuations in the
charge densities of conduction electrons. The result can be a significantfrequency.
shift in
the plasma
64
Chapter 3
Absorption and Dispersion
because of real transitions from d states. The plasma quenched and the reflectance rises. oscillations are The plasma oscillation in silver consists of a collective oscillation, or hybrid resonance, involving both s and d electrons. It can also be thought of as a collective oscillation of the conduction electrons screened by the bound d electrons. The latter viewpoint is illustrated schematically inrise in e 2 (co) (Fig. 3.17)
Fig. 3.20.
and the decomposition of and bound contributions is shown in Fig. 3.22. Although the band structures of copper and silver are qualitatively the same, copper does not exhibit a plasma resonance. The d states in copper lie only 2 eV below the Fermi energy, so that the positive conb tribution of s 1 comes in a frequency region where the negative contribuf tion from e x is of too large a magnitude for & y to reach zero. The difference in color between silver and copper arises from the positionsreflectance of copperis
The
shown
in Fig. 3.21,
the experimental values of s^co) into free
100
\

50


~11
I

\
\\ \\\
x 0.1
\\\
\
\
\N
\6 E(ev)Fig. 3.21
\
\\1012
14
Spectral dependence of the reflectance of
Cu
(lower curve) and Ni (upper curve).
[Cu data from H. Ehrenreich and H.H. Ehrenreich, H. R. Philipp, and D.
R. Philipp, Phys. Rev. 128, 1622 (1962);J.
Ni data from
Olechna, Phys. Rev. 131, 2469 (1963).]
3.3
A
Qualitative
Look
at Real
Metals
65
Fig. 3.22
Decomposition of the experimental values of e^to)(/)
for
Cu
into freeis
and bound
contributionscu,.
and dt:^. The threshold energy for interband transitions [H. Ehrenreich and H. R. Philipp, Phys. Rev. 128, 1622 (1962).]i
indicated by
of the d bands. In
silver,
the dband absorption does not begin until hco
=
4 eV, or at wavelengths less than 3000 A. This is in the ultraviolet, so the reflectance is high throughout the visible. In copper, however, the d bands lie 2 eV below the Fermi energy, so that strong absorption begins at X =
= 6000 A. This wavelength is in the red. Thus, the reflectance of copper decreases in the red spectral region and continues to decrease as the wavelength decreases. Since the reflectance of copper is highest towards the redend of thevisible spectral region,is
copper has a reddish or "copper" color.
The
reflectance of nickel
also
shown
in Fig. 3.21. In nickel
and
in the
other transition metals, the Fermi level intersects the d bands. Interband transitions set in at about 0.3 eV, so it is not feasible to fit the lowfrequency
region to the
Drude model. Interband
transitions cause the reflectance to
drop almost immediately from the limiting reflectance of unity asproaches zero.
w
ap
66
Chapter 3
Absorption and Dispersion
3.4
Photoemission from Copperfirst
look at the optical properties of solids based on some now appropriate to consider some photoemission results which can be readily understood in a qualitative way. Copper presents such a case. Figure 3.23 shows a schematic energy diagram for Cu with a monolayer of Cs to lower the work function from 4.5 eV to 1.55 eV. The application of a monolayer of Cs, other alkali metals, or a compound such as Cs 2 is frequently done in order to lower the work function. There are several reasons for wanting to lower the threshold for photoemission. With practical photocathodes, it is simply the desire to get as high a quantum efficiency as possible at long wavelengths. In band structure studies, a higher quantum efficiency makes it easier to measure photocurrents. Of greater importance, it allows one to probe deeperlying levels with conventional light sources and permits a study of conduction band states between the old vacuum level and the new, lower vacuum level. Of course, it is necessary that the only effect of the applied monolayer be to lower the work function. It must not destroy the fundamental shape of the energy distribution curve (EDC) for the underlying solid. That is something that can be determined only byfairly
Having taken a
simple models,
it is
experiment.
Figure 3.24 shows thelittle
EDC
for
Cu
at four
photon
energies.
There
is
difference
among
the four curves.
Now look at Fig. 3.25 and note the dramatic change in the EDC on going from hv = 3.7 to 3.9 eV. The large spike in the EDC near zero energy results from excitation of d electrons. These states were inaccessible for photoemission with hv 3.7 eV, but are accessible with hv 3.9 eV.Vacuumlevel
sandpstates
d states
Fig. 3.23
Simplified energy
threshold for photoemission from
band diagram for Cu with a surface monolayer of Cs. The s and plike states is 1.55 eV. The threshold for emission
from d
states
is
3.7
eV.
3.5
Quantum Theory
of Absorption and Dispersion
67
Electron energy (eV)
Fig. 3.24
Photoemission from
Cu
with a surface monolayer of Cs. At photon energies
less
than
3.7
eV, electrons excited from d states cannot escape. Thus these curves represent electronss
excited from
and
plike states as illustrated in Fig. 3.23.
[From
C. N. Berglund
and W.
E.
Spicer, Phys. Rev. 136,
A1044
(1964).]
electrons than for
because the density of states is much higher for d and p electrons; there are more d electrons in the outer shells of Cu and the d bands are flatter. Thus, in agreement with optical studies, photoemission shows that the d states in Cu lie 2.1 eV below the Fermi energy {hv = 3.7 eV minus e(j> F = 1.55 eV). Note, though, that by drawing an energy level diagram in the manner of Fig. 3.23, we have avoided any discussion of selection rules. We have been concerned here only with
The
large
peak
resultss
energy conservation.
3.5
Quantum Theory
of Absorption and Dispersion
The polarizability and the dielectric function obtained by a quantum mechanical analysis are of the same form as those obtained with the classical Lorentz model. To show this, we again consider first the interaction of a free atom with an electromagnetic field. We are concerned only with systems initially in their ground state, so that we need consider only the effects of polarization and absorption, not emission.
68
Chapter 3
Absorption and Dispersion
At times
t